- Open Access
A nanomolecular approach to decrease adhesion of biofouling-producing bacteria to graphene-coated material
© Parra et al. 2015
Received: 20 May 2015
Accepted: 16 October 2015
Published: 16 November 2015
Biofouling, the colonization of artificial and natural surfaces by unwanted microorganisms, has an important economic impact on a wide range of industries. Low cost antifouling strategies are typically based on biocides which exhibit a negative environmental impact, affecting surrounding organisms related and not related to biofouling. Considering that the critical processes resulting in biofouling occur in the nanoscale/microscale dimensions, in this work we present a bionanotechnological approach to reduce adhesion of biofilm-producing bacteria Halomonas spp. CAM2 by introducing single layer graphene coatings. The use of this nanomaterial has been poorly explored for antifouling application.
Our study revealed that graphene coatings modify material surface energy and electrostatic interaction between material and bacteria. Such nanoscale surface modification determine an important reduction over resulting bacterial adhesion and reduces the expression levels of genes related to adhesion when bacteria are in contact with graphene-coated material.
Our results demonstrate that graphene coatings reduce considerably adhesion and expression levels of adhesion genes of biofilm-producing bacteria Halomonas spp. CAM2. Hydrophobic-hydrophilic interaction and repulsive electrostatic force dominate the interactions between Halomonas spp. CAM2 and material surface in saline media, impacting the final adhesion process. In addition no bactericide effect of graphene coatings was observed. The effect over biofilm formation is localized right at coated surface, in contrast to other antifouling techniques currently used, such as biocides.
Marine fouling is the accumulation of micro and macroorganisms on underwater surfaces, which provide a favorable mechanism to survive in the environment. The economic impact of fouling on shipping vessels, oceanographic sensors, power plants and aquaculture systems, among others, has been estimated to be in the range of 50 billion euros per year [1–3]. In particular, shipping, fishing and aquaculture industries exhibit extreme fouling cases. On vessels, fouling adds weight to boats and increases hull roughness and hydrodynamic drag, raising fuel consumption by almost 40 %, with the corresponding increase in emissions of greenhouse gases and other pollutants . In aquaculture, settlement of fouling organisms in culture cages causes suffocation of the cultivated species, delaying the time when the cultivated species reaches commercial size . Another singular example is found in boilers cooled with ocean water where the fouling phenomenon causes strong inefficiency in operational parameters and increase in fuel consumption .
Current techniques to prevent (antifouling) and fight fouling (fouling-release) include physical (e.g. heat treatments, pulse-power technology, radioactive coatings, flushing, scrubbing and biological control) and chemical methods (e.g. injectable biocides, chlorine, marine bioactive compounds and other form of bactericide coatings such as copper and copper alloys). Although the choice of the right strategy will depend on the cost and application possibilities, antifouling coatings are probably the most cost-effective method for boats and other surfaces. They are typically based on the controlled release of organic solvents into the environment to kill the colonizing microorganism. However this approach offers a non-localized solution, affecting surrounding organisms related and not related to fouling. As a consequence, the use of certain biocides has been restricted by some countries and in Europe a large amount of data has been gathered as part of the Biocidal Products Directive (BPD, 98/8/EC) .
The critical processes at the biointerface resulting in biofouling occur in the nanoscale/microscale dimensions: it follows therefore that surface properties which could control biofouling need to be on the same length scales . Search for non-biocidal technology to control the economic and environmental problem caused by biofouling has focused, as a result, on modifying physico-chemical and mechanical properties of surfaces (such as surface free energy, wettability, elasticity and surface topography) at the nanoscale to reduce bacterial attachment [9–14]. As far as coatings for marine antifouling applications are concerned, surfaces with low surface energy or with an optimized surface topography (with patterns in the order of micrometer) have shown promising results [13, 15] opening a new avenue for the development of antifouling coatings.
Graphene is a one-atom thick carbon sheet that has emerged as a new carbon compound with multiple applications in a wide range of industrial processes and products. While graphene is a promising candidate in electronic applications, its use for biological applications, such as antifouling, has been poorly explored. There are many reports of bacterial interaction with graphene oxide (GO), formed by micro- or nano-sized flakes of functionalized graphene in powder, solution or coating [16–18], which induces inactivation of bacterial cells upon direct contact by physical and oxidative damage to cell as its antibacterial mechanism [13, 19–22]. Flake size turns out to be a relevant aspect for the reported antibacterial activity of GO, whether this be in suspension or coating [18, 20]. However in the case of single layer graphene sheets grown on Cu, which as GO are one-atom thick, they have surface areas in the centimeter square range. Hence the mechanism of the bacterial interaction must be different in both cases.
In this report we present a physico-chemical and biological approach to reduce fouling formation in its initial growth stage as biofilm, by introducing graphene coatings that reduce bacterial adhesion to coated surfaces. Nanoscale behavior is discussed in the particular case of biofilm-producing Halomonas spp. CAM2, which is used as a model marine bacterium.
Results and discussion
Preparation and characterization of nanostructured modified samples
Micro and nanoscale characterization of as-grown graphene on Cu and graphene transferred onto SiO2 samples was carried out to evaluate their composition, microstructure, topography with atomic resolution, graphitic quality and contamination.
The morphological characterization of graphene grown on Cu and resulting graphene-coated SiO2 samples prior to bacteria contact was screened by SEM, optical microscopy and STM. Wrinkles in CVD graphene grown on Cu are formed by differential thermal expansion, as the metal contracts more than the graphene during post-growth cooling . Such wrinkles are still present after transfer to SiO2 substrate, as can be clearly seen in optical microscopy (Fig. 1d).
In addition, different contrast in certain areas is observed which can be identified as bilayer islands on top of a monolayer background. The surface of SLG transferred onto SiO2 substrates showed micrometric damages in the graphitic membrane due to the transfer procedure, which leaves some SiO2 areas exposed. Clear visualization of the intrinsic hexagonal structure (honeycomb) of graphene transferred onto SiO2 was possible by STM (Fig. 1c, e). Few signs of surface contamination were found by this atomic-resolved technique.
To verify the graphitic quality of graphene coatings we performed microRaman spectroscopy measurements. Multiple areas of each sample were analyzed and representative spectra are shown in Fig. 1f. SLG grown on Cu and SLG transferred onto SiO2 typically display sharp G (1584 cm-1) and 2D (2680–2693 cm-1) bands, with a small G/2D ratio (0.25 and 0.29 respectively). These results are consistent with single layer graphene, according to values reported in literature [26–28].
Graphene coating effects on bacterial adhesion
Graphene coating effects on adhesin gene expression
Graphene coating effects on surface energy, wettability and electrostatic interaction
After overcoming (if) this initial electrostatic repulsion, an even shorter-range hydrophobic interaction (generally when bacteria-surface distance is smaller than 1.5 nm ) have a strong impact on bacterial surface adhesion, a characteristic that is mainly determined by physico-chemical surface properties .
In order to determine the influence of possible hydrophobic characteristics of graphene coatings over bacterial adhesion, we performed contact angle measurements on SiO2 (Fig. 6a), graphene-coated SiO2 (Fig. 6b) and lawns of Halomonas spp. CAM2 previously suspended in water (0 % NaCl) and saline buffer (0.5 % NaCl and 2 % NaCl) (Fig. 6c, d, e respectively).
Contact angles are related to the surface free energies . Hydrophobic coatings are often used to minimize adhesion since they create a larger contact angle between the bacteria’s glue and the surface. This results in less wettability (lower surface energy) and less fouling since the adhesive is not being able to spread across the surface . According to our measurements a transition from hydrophilic surface (contact angle of ~85° ± 0.7) for SiO2 substrate to hydrophobic surface (contact angle of ~95° ± 0.3) for graphene-coated SiO2 is observed.
In addition, cells that possess a hydrophilic character attach preferentially to hydrophilic surfaces (large surface energy), whereas hydrophobic cells prefer hydrophobic surfaces [3, 45]. The hydrophobic-hydrophilic nature of Halomonas spp. CAM2 surface changes as the bacterium grows in different media. Reported response of Halomonas elongata to saline NaCl media, like the one used in the current experiments, displays an enhanced hydrophilicity , which makes the cell more attractive to water molecules in the environment and prevents desiccation. Our contact angle results confirmed such hydrophilic nature of Halomonas spp. CAM2 and a clear trend to increased cell hydrophilicity as a function of salinity of suspension media; 73° for 0 %, 43° for 0.5 % and 32° for 2 % NaCl (Fig. 6c, d, e respectively). In addition these results suggest that the modification from hydrophilic to hydrophobic nature of graphene-coated SiO2 determines the suppression of bacterial attachment for hydrophilic Halomonas spp. CAM2. These results show that both interactions, electrostatic (<5 nm range) and hydrophobic-hydrophilic (<1.5 nm range), are presumably affecting the bacterial attachment process, causing a notorious decrease in adhesin gene expression of Halomonas spp. CAM2, with the corresponding reduction of bacterial adhesion to graphene-coated surfaces.
In this paper we present a nano-biotechnological approach to decrease the attachment of marine bacteria Halomonas spp. CAM2 by introducing graphene coatings. According to our theoretical and experimental results graphene coatings modify surface energy and electrostatic interactions with bacterial cells which determines an important reduction of bacterial adhesion, a relevant parameter involved in biofilm formation and consequent biofouling emergence. This nanoscale surface modification affects the expression of genes related to adhesion that are notoriously decreased when bacteria are in contact with graphene-coated SiO2 surfaces instead of uncoated SiO2 surfaces.
No bactericide effects of graphene-coated SiO2 were observed. Such behavior indicates the effect over biofilm formation is localized right at coated surface, in contrast to other antifouling techniques currently used, such as biocides, that exhibit negative effects over all surrounding aquatic species, not necessarily related to biofilm or biofouling formation. We expect this work will contribute to provide new opportunities for designing effective and environmentally friendly antifouling surfaces based on nanoscale modified materials.
Silicon dioxide coated wafers and commercial CVD graphene grown on Cu was obtained from Graphene Supermarket Company. Graphene and SiO2 samples used in this study were 1 cm2 in area.
Preparation and characterization of Gr/SiO2
Transfer of graphene films grown on Cu to SiO2 substrates was achieved by the poly(methylmethacrylate) (PMMA) assisted method as shown in Fig. 1a. Thin layer of PMMA on graphene on Cu foil was produced by spin-coating. The polymer provides a supportive framework for graphene before the transfer. The underneath Cu substrate is then etched away by an ammonium persulfate ((NH4)2SO8) solution. After the Cu foil is completely dissolved, the floating membrane can be scooped and placed on SiO2. After drying, the polymeric film is dissolved with acetone.
PMMA and ammonium persulfate ((NH4)2SO8) used for graphene transfer procedure were purchased from Sigma Aldrich.
Scanning Tunneling Microscopy (UHV-VT Omicron) was used to characterize nanoscale morphology. Sample preparation before STM measurements consists of 200 °C annealing in UHV for 30 min. Platinum-iridium tips were used for all STM measurements. The experimental data were analyzed by using WSxM software. Scanning Electron Microscopy (SEM) images were recorded using a Carl Zeiss microscope (EVO MA-10) to characterize microscale morphology and qualitative bacterial adhesion. MicroRaman measurements (Renishaw, 532 nm laser) were used to characterize quality of as-grown graphene and transferred graphene onto SiO2. Contact angle measurements were performed to characterize surface hydrophobicity of coated and uncoated Cu samples. A drop of milliQ water (2μL) was placed on the surface of graphene-coated SiO2 and uncoated samples and images were immediately captured using a high-resolution camera. Bacterial hydrophobicity was measured following standard methods  with some modifications. A bacterial strain suspended in 40 mL of water, 0.5 % NaCl and 2 % NaCl were filtered on a micropore cellulose nitrate filter (pore size 0.45 μm, Sartorius Stedim Biotech, Germany) by filtration of the suspension using negative pressure. The filters with a bacteria film were dried at room temperature during 90 min in order to obtain a stable water contact angle measured by sessile drop method using 1 μL of distilled. The contact angle was measured based on image analysis  using the image processing software Image J with the plug-in Drop Shape Analysis based on B-spline snakes algorithm developed by .
Bacterial strain isolation
A marine strain Halomonas spp. CAM2 was used in the biofilm formation assays. Bacteria was previously isolated from illness larvae of the Chilean scallop Argopecten purpuratus Lamarck, 1891 (bivalvia, pectinidae) and characterized . Stock cultures of the CAM2 strain were maintained at 4 °C on Tryptic soy agar (Difco) supplemented with NaCl (2 %), and subcultured every 2 weeks. For long-term preservation, CAM2 strain cultures were frozen at −80 °C in Tryptic soy broth (Difco) supplemented with 2 % NaCl (w/v) and 20 % glycerol (v/v) . When required, frozen cultures were recovered by streaking onto Tryptic soy agar plates (Difco) supplemented with NaCl (2 %), which were incubated at 20 °C for 24 h.
Bacteria culture and exposure to Gr/SiO2
Surfaces used for biofilms growth were sterilized by rinsing several times with ethanol and sterilized DI water. Bacterial adhesion assays on partially graphene-coated SiO2 were performed in petri dishes. TSA Agar plates were inoculated with freshly growing cells of Halomonas spp. CAM2, so that a lawn of bacteria was grown. After 48 h incubation at 25 °C a half of the surface containing bacteria (in exponential to early stationary phase) was harvested and suspended in 10 ml of sterile saline buffer (0.5 % NaCl). This volume was poured on pieces of 1 cm2 of Gr/SiO2 and SiO2 and incubated for 72 h at 20 °C. An aliquot was removed in order to determine the cell concentration by dilution plating. All experiments were run in triplicate.
Bacterial adhesion study
Analysis of bacterial adhesion was conducted in order to evaluate morphology and viability of microorganisms. For SEM characterization bacteria were fixed on samples with 3 % (v/v) glutaraldehyde and dehydrated by washing with a graded ethanol series (from 10 to 100 %), followed by critical-point drying and gold coating.
Distribution of bacteria on Gr/SiO2 or SiO2 surfaces was determined directly in situ. For epifluorescence analysis Gr/SiO2 or SiO2 pieces were submerged into solution provided by standard LIVE/DEAD BacLight bacterial viability kit (0.01 mM of Syto9 and 0.06 mM of propidium iodide). Samples were kept dark during 15 min and then observed by epifluorescence microscopy Olympus × 71.
Expression of adhesion genes
Sequences of oligonucleotide primers used for qPCR
Amplicon size (bp)
For RNA isolation, SiO2 surfaces with and without graphene were washed twice with phosphate buffer. Bacteria were scrapped from samples surface with a sterile cotton swab and were stored at −80 °C awaiting RNA isolation . Bacterial RNA was extracted using TRIzol reagent (Ambion by Lifetechnologies).
Samples were defrosted, and genes were extracted using chloroform. RNA was recovered by precipitation with ethanol 70 % and was load on Qiagen RNeasy minElute spin column following manufacturer’s instructions.
RNA quantity was determined by measuring the absorbance at 260 nm using a Nanodrop spectrophotometer ND-1000 (Thermo Fisher Scientific). Contaminated genomic DNA was removed by TURBO DNA-free kit (ambion by lifetechnologies). Further, total RNA samples were analyzed for the presence of DNA contamination by qRT-PCR using 16S rRNA target.
Purified RNA was converted to cDNA using RevertAid™ first strand cDNA synthesis kit (Fermentas) with random hexamer primers according to manufacturer’s instructions.
Real time PCR was performed according to the protocol of the SYBR Green/Rox qPCR Master Mix (Fermentas) with Stratagene Mx3000P real-time PCR system (Stratagene); 16S mRNA levels were used for normalization.
Amplification courses in all genes included the following 3 steps: (1) 1 cycle of an initial denaturation for 10 min at 95 °C, (2) 40 cycles of an initial denaturation for 30 s at 95 °C. Annealing for 1 min at 55 °C and extension for 30 s at 72 °C and, (3) 1 cycle of an initial denaturation for 1 min at 95 °C, annealing for 30 s at 55 °C a final extension for 30 s at 95 °C.
Relative quantification of each target gene (F7SSV5, F7SSV2, G4F3Q7, AlgC) encoding for adhesin in each experimental sample, and control versus reference gene (rDNA16S) was performed in according with Livak Eq. 1: relative expression ratio (R) = 2−[ΔCt sample − ΔCt control] = 2−ΔΔCt.
CP, FD, ED, RR, CR collected research data. CP, FD, RH, CR and PV analyzed the data. CP, CR and PV wrote this article. All authors read and approved the final manuscript.
This research was supported by Innova Corfo L1 13IDL1-25496, Chilean Government. PV is grateful for access to Sherwin William facilities, Santiago, Chile.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Azis PKA, Al-Tisan I, Sasikumar N. Biofouling potential and environmental factors of seawater at the desalination plant intake. Desalination. 2001;135:69–82.View ArticleGoogle Scholar
- Fitridge I, Dempster T, Guenther J, de Nys R. The impact and control of biofouling in marine aquaculture: a review. Biofouling. 2012;28:649–69.View ArticleGoogle Scholar
- Tuson HH, Weibel DB. Bacteria-surface interactions. Soft Matter. 2013;9:4368–80.View ArticleGoogle Scholar
- Townsin RL. The ship hull fouling penalty. Biofouling. 2003;19:9–15.View ArticleGoogle Scholar
- Greene JK, Grizzle RE. Successional development of fouling communities on open ocean aquaculture fish cages in the western Gulf of Maine. Aquaculture. 2007;262:289–301.View ArticleGoogle Scholar
- Pronobis M. The influence of biomass co-combustion on boiler fouling and efficiency. Fuel. 2006;85:474–80.View ArticleGoogle Scholar
- Thomas KV, Brooks S. The environmental fate and effects of antifouling paint biocides. Biofouling. 2010;26:73–88.View ArticleGoogle Scholar
- Szewczyk P. The role of nanotechnology in improving marine antifouling coatings. Zesz Nauk/Akad Morska Szczecinie. 2010;24:118–23.Google Scholar
- Beigbeder PD, Conlan SL, Mutton R, Clare AS, Pettitt ME, Callow ME, et al. Preparation and characterization of silicone-based coatings filled with carbon nanotubes and natural sepiolite and their application as marine fouling-release coating. Biofouling. 2008;24:291.View ArticleGoogle Scholar
- Adiga SP, Jin C, Curtiss LA, Monteiro-Riviere NA, Narayan RJ. Nanoporous membranes for medical and biological applications. Nanomed Nanobiotechnol. 2009;1:568–81.View ArticleGoogle Scholar
- Callow JA, Callow ME. Trends in the development of environmentally friendly fouling-resistant marine coatings. Nat Commun. 2011;2:1–10.View ArticleGoogle Scholar
- Sheet I, Holail H, Olama Z, Kabbani A, Hines M. The antibacterial activity of graphite oxide, silver, impregnated graphite oxide with silver and GO-coated sand nanoparticles against waterborne pathogenic E. coli BL21. Int J Curr Microbiol App Sci. 2013;2:1–11.Google Scholar
- Banerjee I, Pangule RC, Kane RS. Antifouling coatings: recent developments in the design of surfaces that prevent fouling by proteins, bacteria, and marine organisms. Adv Mater. 2011;23:690–718.View ArticleGoogle Scholar
- Krishnan S, Weinman CJ, Ober CK. Advances in polymers for anti-biofouling surfaces. J Mater Chem. 2008;18:3405–13.View ArticleGoogle Scholar
- Petronis S, Berntsson K, Gold J, Gatenholm P. Design and microstructuring of PDMS surfaces for improved marine biofouling resistance. J Biomater Sci Polym Ed. 2000;11:1051.View ArticleGoogle Scholar
- Yu L, Zhang Y, Zhang B, Liu J, Zhang H, Song C. Preparation and characterization of HPEI-GO/PES ultrafiltration membrane with antifouling and antibacterial properties. J Membr Sci. 2013;444:452–62.View ArticleGoogle Scholar
- Yu L, Zhang Y, Zhang B, Liu J. Enhanced antibacterial activity of silver nanoparticles/halloysite nanotubes/graphene nanocomposites with sandwich-like structure. Sci Rep. 2014;4:4551–5.Google Scholar
- Perrault F, de Faria AF, Nejati S, Elimelech M. Antimicrobial properties of graphene oxide nanosheets: why size matters. ACS Nano. 2015;9:7226–36.View ArticleGoogle Scholar
- Perreault F, de Faria FA, Elimelech M. Environmental applications of graphene-based nanomaterials. Chem Soc Rev. 2015;44:5861–96.View ArticleGoogle Scholar
- Perreault F, Tousley ME, Elimelech M. Thin-film composite polyamide membranes functionalized with biocidal graphene oxide nanosheets. Environ Sci Technol Lett. 2014;1:71–6.View ArticleGoogle Scholar
- Romero-Vargas Cartrillón S, Perrault F, de Faria FA, Elimelech M. Interaction of graphene oxide with bacterial cell membranes: insights from force spectroscopy. Environ Sci Technol Lett. 2015;2:112–7.View ArticleGoogle Scholar
- Al-Thani RF, Patan NK, Al-Maadeed MA. Graphene oxide as antimicrobial against two gram-positive and two gram-negative bacteria in addition to one fungus. Online J Biol Sci. 2014;14:230–9.View ArticleGoogle Scholar
- Park J, Lee J, Liu L, Clark KW, Durand C, Park C, et al. Spatially resolved one-dimensional boundary states in graphene–hexagonal boron nitride planar heterostructures. Nat Commun. 2014;5:5403.View ArticleGoogle Scholar
- Yu Q, Jauregui LA, Wu W, Colby R, Tian J, Su Z, et al. Control and characterization of individual grains and grain boundaries in graphene grown by chemical vapor deposition. Nat Mater. 2011;10:443–9.View ArticleGoogle Scholar
- Calado VE, Schneider GF, Theulings AMMG, Dekker C, Vandersype LMK. Formation and control of wrinkles in graphene by the wedging transfer method. Appl Phys Lett. 2012;10:103116.View ArticleGoogle Scholar
- Li X, Cai W, An J, Kim S, Nah J, Yang D, et al. Large-area synthesis of high-quality and uniform graphene films on copper foils. Science. 2009;324:1312–4.View ArticleGoogle Scholar
- Ferrari AC, Meyer JC, Scardaci V, Casiraghi C, Lazzeri M, Mauri F, et al. Raman spectrum of graphene and graphene layers. Phys Rev Lett. 2006;97:187401–5.View ArticleGoogle Scholar
- Reina A, Jia X, Ho J, Nezich D, Son H, Bulovic V, et al. Large area, few-layer graphene films on arbitrary substrates by chemical vapor deposition. Nano Lett. 2008;9:30–5.View ArticleGoogle Scholar
- Parra C, Montero-Silva F, Henríquez R, Flores M, Garín C, Ramírez C, et al. Suppressing bacterial interaction with copper surfaces through graphene and hexagonal-boron nitride coatings. ACS Appl Mater Interfaces. 2015;7:6430–7.View ArticleGoogle Scholar
- Cai L, Tan D, Aibaidula G, Dong XR, Chen JC, Tian WD, Chen GQ. Comparative genomics study of polyhydroxyalkanoates (PHA) and ectoine relevant genes from Halomonas sp. TD01 revealed extensive horizontal gene transfer events and co-evolutionary relationships. Microb Cell Fact. 2011;10:88–103.View ArticleGoogle Scholar
- Lin Y, Fan H, Hao X, Johnstone L, Hu Y, Wei G, et al. Draft genome sequence of Halomonas sp. strain HAL1, a moderately halophilic arsenite-oxidizing bacterium isolated from gold-mine soil. J Bacteriol. 2012;194:199–200.View ArticleGoogle Scholar
- Zielinski NA, Chakrabarty AM, Berry A. Characterization and regulation of the Pseudomonas aeruginosa algC gene encoding phosphomannomutase. J Biol Chem. 1991;266:9754–63.Google Scholar
- Gottenbos B, Busscher HJ, Van Der Mei HC, Nieuwenhuis P. Pathogenesis and prevention of biomaterial centered infections. J Mater Sci Mater Med. 2002;13:717–22.View ArticleGoogle Scholar
- Romero HE, Shen N, Joshi P, Gutierrez HR, Tadigadapa SA, Sofo JO, Eklund PC. n-type behavior of graphene supported on Si/SiO2 substrates. ACS Nano. 2008;2:2037–44.View ArticleGoogle Scholar
- Hogt AH, Dankert J, Feijen J. Adhesion of coagulase-negative Staphylococci to methacrylate polymers and copolymers. J Biomed Mater Res. 1986;20:533–45.View ArticleGoogle Scholar
- Elimelech M, Gregory J, Jia X, Williams R. Particle deposition and aggregation. Williams RA, Woburn MA, editors. Oxford: Butterworth-Heinemann; 1995.Google Scholar
- Itoh H, Sakuma H. Dielectric constant of water as a function of separation in a slab geometry: a molecular dynamics study. J Chem Phys. 2015;142:184703.View ArticleGoogle Scholar
- Linke D, Goldman A. Bacterial adhesion: chemistry, biology and physics. Berlin: Springer; 2011.View ArticleGoogle Scholar
- Ducker WA, Senden TJ, Pashley RM. Measurement of forces in liquids using a force microscope. Langmuir. 1992;8:1831–6.View ArticleGoogle Scholar
- Deshpande Bao, Miao F, Lau CN, LeRoy BJ. Spatially resolved spectroscopy of monolayer graphene on SiO2. Phys Rev B. 2009;79:205411–6.View ArticleGoogle Scholar
- Bruinsma GM, van der Mei HC, Busscher H. Bacterial adhesion to surface hydrophilic and hydrophobic contact lenses. Biomaterials. 2001;22:3217–24.View ArticleGoogle Scholar
- Busscher HJ, Weerkamp AH. Specific and non-specific interactions in bacterial adhesion to solid substrata. FEMS Microbiol Lett. 1987;46:165–73.View ArticleGoogle Scholar
- Bos R, Van der Mei HC, Busscher HJ. Physico-chemistry of initial microbial adhesive interactio–its mechanisms and methods for study. FEMS Microbiol Rev. 1999;23:179–230.View ArticleGoogle Scholar
- Chapman J, Sullivan T, Regan F. Nanoparticles in anti-microbial materials: use and characterization. Cambridge: The Royal Society of Chemistry; 2012. p. 40–8.Google Scholar
- Montanaro L, Campoccia D, Rizzi S, Donati ME, Breschi L, Prati C, Arciola CR. Evaluation of bacterial adhesion of Streptococcus mutants in dental restorative materials. Biomaterials. 2004;25:4457–63.View ArticleGoogle Scholar
- Hart DJ, Vreeland RH. Changes in the hydrophobic-hydrophilic cell surface character of Halomonas elongata in response to NaCl. J Bacteriol. 1988;170:132–5.Google Scholar
- Ramírez C, Gallegos I, Ihl M, Bifani V. Study of contact angle, wettability and water vapor permeability in carboxymethylcellulose (CMC) based film with murta leaves (Ugni molinae Turcz) extract. J Food Eng. 2012;109:424–9.View ArticleGoogle Scholar
- Stalder AF, Kulik G, Sage D, Barbieri L, Hoffmann P. A snake-based approach to accurate determination of both contact points and contact angles. Colloids Surf A. 2006;286:92–103.View ArticleGoogle Scholar
- Rojas R. Pathogenicity of a highly exopolysaccharide-producing Halomonas strain causing epizootics in larval cultures of the chilean scallop Argopecten purpuratus. Microb Ecol. 2009;57:129–39.View ArticleGoogle Scholar
- Sambrook J, Russell DW. Molecular cloning: A laboratory manual. New York: Cold Spring Harbor Laboratory Press; 2012.Google Scholar
- Atshan SS, Shamsudin MN, Karunanidhi A, van Belkum A, Lung LT, Sekawi Z, Nathan JJ, Ling KH, Seng JS, Ali AM, Abduljaleel SA, Hamat RA. Quantitative PCR analysis of genes expressed during biofilm development of methicillin resistant Staphylococcus aureus (MRSA). Infect Genet Evol. 2013;18:106–12.View ArticleGoogle Scholar